Dimensional reduction upon calcium incorporation in Cs0.3(Ca0.3Ln0.7)PS4 and Cs0.5(Ca0.5Ln0.5)PS4
Klepov, Vladislav V.; Kocevski, Vancho; Besmann, Theodore M.; zur Loye, Hans-Conrad; CrystEngComm 23 (2021) 831–840; doi:10.1039/D0CE01524E

data_7241715
_publ_section_title
;
 Dimensional reduction upon calcium incorporation in Cs0.3(Ca0.3Ln0.7)PS4
 and Cs0.5(Ca0.5Ln0.5)PS4
;
_journal_issue                   4
_journal_name_full               CrystEngComm
_journal_page_first              831
_journal_page_last               840
_journal_paper_doi               10.1039/D0CE01524E
_journal_volume                  23
_journal_year                    2021
_chemical_formula_sum            'Ca0.3 Cs0.3 P Pr0.7 S4'
_chemical_formula_weight         309.74
_space_group_crystal_system      trigonal
_space_group_IT_number           166
_space_group_name_Hall           '-R 3 2"'
_space_group_name_H-M_alt        'R -3 m :H'
_audit_creation_method           SHELXL-2018/1
_audit_update_record
;
2020-10-14 deposited with the CCDC.	2020-12-01 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            18
_cell_length_a                   16.4968(4)
_cell_length_b                   16.4968(4)
_cell_length_c                   13.5795(3)
_cell_measurement_reflns_used    9674
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      36.32
_cell_measurement_theta_min      3.22
_cell_volume                     3200.47(13)
_computing_structure_refinement  'SHELXL-2018/1 (Sheldrick, 2018)'
_diffrn_ambient_temperature      300(2)
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Bruker D8 QUEST'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0278
_diffrn_reflns_av_unetI/netI     0.0059
_diffrn_reflns_Laue_measured_fraction_full 0.985
_diffrn_reflns_Laue_measured_fraction_max 0.988
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            68364
_diffrn_reflns_point_group_measured_fraction_full 0.985
_diffrn_reflns_point_group_measured_fraction_max 0.988
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.489
_diffrn_reflns_theta_min         3.222
_exptl_absorpt_coefficient_mu    7.845
_exptl_absorpt_correction_T_max  0.3874
_exptl_absorpt_correction_T_min  0.2950
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
 Reference: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10.
;
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.893
_exptl_crystal_description       block
_exptl_crystal_F_000             2570
_exptl_crystal_size_max          0.100
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.050
_refine_diff_density_max         3.370
_refine_diff_density_min         -4.618
_refine_diff_density_rms         0.203
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.085
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     43
_refine_ls_number_reflns         902
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.085
_refine_ls_R_factor_all          0.0327
_refine_ls_R_factor_gt           0.0327
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0473P)^2^+56.5187P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0859
_refine_ls_wR_factor_ref         0.0859
_reflns_Friedel_coverage         0.000
_reflns_number_gt                902
_reflns_number_total             902
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0ce01524e2.cif
_cod_data_source_block           Pr07
_cod_depositor_comments
'Adding full bibliography for 7241712--7241724.cif.'
_cod_original_cell_volume        3200.47(17)
_cod_original_formula_sum        'Ca0.30 Cs0.30 P Pr0.70 S4'
_cod_database_code               7241715
_shelx_shelxl_version_number     2018/1
_shelx_estimated_absorpt_t_min   0.508
_shelx_estimated_absorpt_t_max   0.695
_shelx_res_checksum              64628